Nano Express | Open | Published:
Comparative Study of Negative Capacitance Field-Effect Transistors with Different MOS Capacitances
Nanoscale Research Lettersvolume 14, Article number: 171 (2019)
We demonstrate the negative capacitance (NC) effect of HfZrOx-based field-effect transistors (FETs) in the experiments. Improved IDS, SS, and Gm of NCFET have been achieved in comparison with control metal oxide semiconductor (MOS) FET. In this experiment, the bottom MIS transistors with different passivation time are equivalent to the NC devices with different MOS capacitances. Meanwhile, the electrical properties of NCFET with 40 min passivation are superior to that of NCFET with 60 min passivation owing to the good matching between CFE and CMOS. Although SS of sub-60 mV/decade is not achieved, the non-hysteretic transfer characteristics beneficial to the logic applications are obtained.
With the scaling down of transistor, the integration level of integrated circuit (IC) is continuous growing. An accompanying power dissipation problem is urgent to be solved. In order to circumvent this problem, the operation voltage of the transistor should be reduced . The subthreshold swing (SS) of MOSFET cannot be below 60 mV/decade at room temperature, which restricts the reduction of threshold voltage VTH and supply voltage VDD . Many efforts have been devoted to the research and the development of devices with novel transport and switching mechanisms to beat the Boltzmann limit, including negative capacitance field-effect transistor (NCEFT) [3, 4], resistive gate FET , nano-electro mechanical FET (NEMFET) [6, 7], impact ionization metal-oxide-semiconductor (I-MOS) [8, 9], and tunneling FET [10, 11]. Among them, NCFET has aroused much attention because it can achieve a steep SS without losing the drive current [12,13,14,15]. Doped HfO2 (e.g., HfZrOx (HZO) and HfSiOx) has been widely used in NCFETs [4, 16, 17]; it is compatible with the CMOS process . A theoretical study has shown that the undesired hysteresis occurs due to unmatched ferroelectric capacitance CFE to underlying MOS capacitance CMOS in NCFET . However, the effect of matching between CFE and CMOS on the electrical characteristics of NCFETs is still a concern in the experiments.
In this work, the electrical characteristics of NC Ge FETs with different MOS capacitances are studied based on the different matching between CFE and CMOS. Although SS less than 60 mV/decade does not appear, the hysteresis-free transfer characteristics and better electrical properties are obtained. Apparent peaks of CFE versus VFE curves demonstrate NC effect of HZO based NCFETs. The better matching of CFE and CMOS contributes to steeper SS and higher on current, which is beneficial to the logic applications.
The key fabrication process of Ge NCFETs is shown in Fig. 1a. Four-inch n-Ge(001) wafers with a resistivity of 0.088–0.14 Ω·cm were used as the starting substrates. After pre-gate cleaning, Ge wafers were loaded into an ultra-high vacuum chamber for surface passivation using Si2H6. Two passivation durations of 40 and 60 min were used. Then, TaN/HZO/TaN/HfO2 stack was deposited. The thicknesses of the HfO2 dielectric layer and HZO FE layer are 4.35 and 4.5 nm, respectively. After gate patterning and etching, source/drain (S/D) regions were implanted using boron ions (B+) at an energy of 30 keV and a dose of 1 × 1015 cm−2. S/D metal Nickel was formed using a lift-off process. Finally, rapid thermal annealing at 450 °C for 30 s was carried out. Control MOSFET with TaN/HfO2 stack was also fabricated. Figures 1b and c show the schematics of fabricated NCFET and control MOSFET, respectively. The internal metal gate in the fabricated NCFET counterbalances the potential at the channel surface, which is called the MFMIS structure.
Results and Discussion
Figure 2a plots the measured IDS-VGS curves of a pair of NCFET and control MOSFET with 40 min surface passivation. Both devices have a gate length LG of 3.5 μm. The NC device with 40 min passivation has a significantly improved IDS than the control MOSFET. The transfer curves of NCFET exhibit a non-hysteretic feature. Point SS versus IDS curves in Fig. 2b show that the NC transistor has improved SS over the control device, although SS of sub-60 mV/decade does not appear. Figure 2c shows that NC transistor obtains a significantly boosted linear transconductance Gm over the control device at VDS of − 0.05 V. Figure 3 compares the electrical performances of NCFET and control MOSFET with surface passivation for 60 min. Similarly, the IDS, point SS and Gm of NCFET are superior to that of control MOSFET.
Figure 4a shows the statistical results of the drive current of NCFETs and control MOSFETs at VDS of − 0.05 V and VGS-VTH = − 1.0 V. NCFETs demonstrate 18.7% and 35.6% improvement in IDS for the 60 min and 40 min surface passivation, respectively, in comparison with the control devices. It is speculated that the NCFETs passivated for 40 min have a better matching between CMOS and CFE over the NC devices with 60 min. Figure 4b shows that NCFETs obtain 26.4% and 51.3% improvement in maximum transconductance Gm,max for 60 min and 40 min surface passivation, respectively, in comparison with the control devices. It is seen that the control MOSFETs with surface passivation for 40 min have a higher IDS and Gm,max than the devices passivated for 60 min, which is due to the larger CMOS induced by the smaller equivalent oxide thickness (EOT). The internal metal gate provides an equipotential plane; the device can be equivalently modeled as a capacitive voltage divider. The total capacitance CG is a series of CFE and CMOS. The internal gate voltage is amplified owing to the NC effect. The internal voltage amplification coefficient β = ∣ CFE ∣ / ∣ CFE ∣ − CMOS gets the maximum when |CMOS| = |CFE| [20, 21]. Achieving the optimized matching of CFE and CMOS is the prerequisite of the improvement of on current.
The extracted Vint versus gate voltage VGS curves are shown in Fig. 5a. Vint of NC transistor can be extracted on account of the hypothesis that IDS-Vint curve of NC transistor is exactly identical with IDS-VGS curve of the control device. The internal voltage amplification coefficient dVint/dVGS is shown in Fig. 5b. dVint/dVGS > 1 is achieved in the wide sweeping range of VGS for the NCFET with 40 min surface passivation, contributing to a steeper SS than the control device during the measuring process, which is due to the local polarization switching . It is consistent with the aforementioned results in Fig. 2b. For the NCFET with 60 min passivation, the internal voltage amplification coefficient dVint/dVGS > 1 is achieved during the range of VGS < 0 V for the double sweeping of VGS, which is in agreement with the elevated SS in Fig. 3b.
Figure 6a shows the extracted CMOS versus VGS curves for NC transistor, which is relying on the Vint-VGS in Fig. 5a and the CG-VGS curves of control MOSFETs. The extracted CMOS is in good agreement with the measured CG. Hence, the validity of the calculation method is demonstrated. The CFE and CMOS versus VFE curves are depicted in Fig. 6b. From the initiation of NC effect, the absolute value of negative CFE of the transistor exceeds CMOS for double sweeping of VGS all the time in Fig. 6b. |CFE| > CMOS and CFE < 0 can cause hysteresis-free characteristics, and the matching of CMOS and CFE is beneficial to the logic applications [23, 24]. Hysteresis-free characteristics in Figs. 2a and 3a are observed attributed to all the domain matching and inhibited charge trapping . The stable polarization switching is responsible for the non-hysteretic characteristics . Furthermore, the large internal gate gain dVint/dVG > 1 is ascribed to the slight discrepancy between |CFE| and CMOS in the subthreshold region, resulting in the steep SS of NC device. Meanwhile, there is a better matching between CFE and CMOS for the NCFET with 40 min passivation than the NCFET with 60 min passivation. Thus, this provides direct evidence to indicate that the NCFET with 40 min passivation possesses a better electrical performance than the NCFET with 60 min passivation. The FE polarization changes the VFE; hence the charge of FE varies. The total charge multiplies, which is attributed to the FE polarization besides the increment of VGS. In other words, for the given VGS, the charge in the channel increases so the IDS improves. As a consequence, the steep SS of transfer characteristic appears in the experiments.
The hysteresis-free transfer characteristics are obtained for the NCFETs with 40 and 60 min passivation. NC Ge pFETs with 40 min passivation have better electrical characteristics than the NC device with 60 min passivation in experiments. We also demonstrate the NC effect of HZO based NCFETs. For NCFETs, the steep SS and dVint/dVGS > 1 are obtained. The NCFET with 40 min passivation has achieved a good matching between CFE and CMOS, which contributes to the non-hysteretic characteristics. The different NC behaviors are considered to be related to the microscopic domain wall switching in the FE thin films.
Availability of Data and Materials
The datasets supporting the conclusions of this article are included in the article.
- B+ :
- E OT :
Equivalent oxide thickness
Impact ionization metal-oxide-semiconductor
Metal oxide semiconductor
Negative capacitance field-effect transistor
Nano-electro mechanical FET
Ionescu AM, Michielis D, Dagtekin N, Salvatore G, Cao l AR, Bartsch S (2011) Ultra low power: emerging devices and their benefits for integrated circuits. In: IEEE International Electron Devices Meeting, Washington. https://doi.org/10.1109/IEDM.2011.6131563
Avci UE, Morris DH, Young IA (2015) Tunnel field-effect transistors: prospects and challenges. IEEE Journal of the Electron Devices Society 3:88–95
Chung W, Meng S, Peide DY (2017) Hysteresis-free negative capacitance germanium CMOS FinFETs with bi-directional sub-60 mV/dec. In: IEEE International Electron Devices Meeting, San Francisco. https://doi.org/10.1109/IEDM.2017.8268395
Kwon D, Chatterjee K, Tan AJ, Yadav AK, Zhou H, Sachid AB, Reis RD, Hu C, Salahuddin S (2017) Improved subthreshold swing and short channel effect in FDSOI n-channel negative capacitance field effect transistors. IEEE Electron Device Lett 39:300–303
Huang Q, Huang R, Pan Y, Tan S, Wang Y (2014) Resistive-gate field-effect transistor: a novel steep-slope device based on a metal-insulator-metal-oxide gate stack. IEEE Electron Device Letters 35:877–879
Kam H, Lee DT, Howe RT, King T-J (2005) A new nano-electro-mechanical field effect transistor (NEMFET) design for low-power electronics. In: IEEE International Electron Device Meeting, Washington, DC. https://doi.org/10.1109/IEDM.2005.1609380
Abele N, Fritschi N, Boucart K, Casset F, Ancey P, Ionescu AM (2005) Suspended-gate MOSFET: bringing new MEMS functionality into solid-state MOS transistor. In: IEEE International Electron Device Meeting, Washington, DC. https://doi.org/10.1109/IEDM.2005.1609384
Choi WY, Song JY, Lee JD, Park YJ, Park B-G (2005) 100-nm n-/p-channel I-MOS using a novel self-aligned structure. IEEE Electron Device Lett 26:261–263
Ramaswamy S, Kumar MJ (2014) Junction-less impact ionization MOS: proposal and investigation. IEEE Trans Electron Devices 61:4295–4298
Han G, Wang Y, Liu Y, Zhang C, Feng Q, Liu M, Zhao S, Cheng B, Zhang J, Hao Y (2016) GeSn Quantum Well P-Channel Tunneling FETs Fabricated on Si(001) and (111) with improved subthreshold swing. IEEE Electron Device Lett 37:701–704
Ionescu AM, Riel H (2011) Tunnel field-effect transistors as energy-efficient electronic switches. Nature 479:329–337
Garam K, Lee J, Kim JH, Kim S (2019) High on-current Ge-channel heterojunction tunnel field-effect transistor using direct band-to-band tunneling. Micromachines 10:E77
Zhou J, Han G, Li Q, Peng Y, Lu X, Zhang C, Zhang J, Sun Q, Zhang D, Hao Y (2016) Ferroelectric HfZrOx Ge and GeSn PMOSFETs with sub-60 mV/decade subthreshold swing, negligible hysteresis, and improved IDS. In: IEEE International Electron Devices Meeting, San Francisco. https://doi.org/10.1109/IEDM.2016.7838401
Zhou J, Peng Y, Han G, Li Q, Liu Y, Zhang J, Liao M, Sun Q, Zhang D, Zhou Y, Hao Y (2018) Hysteresis reduction in negative capacitance Ge PFETs enabled by modulating ferroelectric properties in HfZrOx. IEEE J Electron Devices Soc 6:41–48
Wu J, KanYang R, Han G, Zhou J, Liu Y, Wang Y, Peng Y, Zhang J, Sun Q, Zhang D, Hao Y (2018) Nonideality of negative capacitance Ge field-effect transistors without internal metal gate. IEEE Electron Device Lett 39:614–617
Sharma P, Zhang J, Ni K, Datta S (2018) Time-resolved measurement of negative capacitance. IEEE Electron Device Letters 39:272–275
Li KS, Chen P-G, Lai TY, Lin CH, Cheng C-C, Chen CC, Liao M-H, Lee MH, Chen MC, Sheih JM, Sheih WK, Yeh WK, Yang FL, Salahuddin S, Hu C (2015) Sub-60 mV-Swing negative-capacitance FinFET without hysteresis. In: IEEE International Electron Devices Meeting, Washington, DC. https://doi.org/10.1109/IEDM.2015.7409760
Lee MH, Lin J-C, Wei Y-T, Chen C-W, Tu W-H, Zhuang H-K, Tang M (2013) Ferroelectric negative capacitance hetero-tunnel field-effect-transistors with internal voltage amplification. In: IEEE International Electron Devices Meeting, Washington, DC. https://doi.org/10.1109/IEDM.2013.6724561
Khan AI, Chatterjee K, Duarte JP, Lu Z, Sachid A, Khandelwal S, Ramesh R, Hu C, Salahuddin S (2016) Negative capacitance in short-channel FinFETs externally connected to an epitaxial ferroelectric capacitor. IEEE Electron Device Letters 37:111–114. https://doi.org/10.1109/LED.2015.2501319
Khan AI, Yeung CW, Hu C, Salahuddin S (2011) Ferroelectric negative capacitance MOSFET: capacitance tuning & antiferroelectric operation. In: IEEE International Electron Devices Meeting, Washington, DC. https://doi.org/10.1109/IEDM.2011.6131532
Yueng CW, Khan AI, Sarker A, Salahuddin S, Hu C (2013) Low power negative capacitance FETs for future quantum-well body technology. In: international symposium on VLSI Technology, Hsinchu. https://doi.org/10.1109/VLSI-TSA.2013.6545648
Li X, Toriumi A (2018) Direct relationship between sub-60 mV/dec subthreshold swing and internal potential instability in MOSFET externally connected to ferroelectric capacitor. In: IEEE International Electron Devices Meeting. https://doi.org/10.1109/IEDM.2018.8614703
Pahwa G, Dutta T, Agarwal A, Chauhan YS (2017) Compact model for ferroelectric negative capacitance transistor with MFIS structure. IEEE Trans Electron Devices 64:1366–1374
Khan AI, Radhakrishna U, Salahuddin S, Antoniadis D (2017) Work function engineering for performance improvement in leaky negative capacitance FETs. IEEE Electron Device Letters 38:1335–1338
Hoffmann M, Max B, Mittmann T, Schroeder U, Slesazeck S, Mikolajick T (2018) Demonstration of high-speed hysteresis-free negative capacitance in ferroelectric Hf0.5Zr0.5O2. In: IEEE International Electron Devices Meeting. https://doi.org/10.1109/IEDM.2018.8614677
Zhou J, Han G, Xu N, Li J, Peng Y, Liu Y, Zhang J, Sun Q, Zhang D, Hao Y (2019) Incomplete dipoles flipping produced near hysteresis-free negative capacitance transistors. IEEE Electron Device Lett 40:329–332
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.